LMucko/crystallography-open-database huggingface dataset:
Reactions of diisopropylcarbodiimide with dehalogenation products of (disopropylamino) difluoroborane
Maringgele, W.; Stalke, D.; Heine, A.; Meller, A.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 867–881; doi:

data_4030344
_publ_section_title
;
 Reactions of diisopropylcarbodiimide with dehalogenation products of
 (disopropylamino) difluoroborane
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              867
_journal_page_last               881
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'C14 H30 N4'
_chemical_formula_weight         254.42
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                84.68(2)
_cell_angle_beta                 76.44(3)
_cell_angle_gamma                71.06(2)
_cell_formula_units_Z            4
_cell_length_a                   9.886(4)
_cell_length_b                   12.715(6)
_cell_length_c                   14.851(7)
_cell_volume                     1716.2(14)
_diffrn_ambient_temperature      153
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    0.06
_exptl_crystal_density_diffrn    0.985
_exptl_crystal_F_000             568
_refine_ls_number_parameters     342
_refine_ls_number_reflns         3488
_refine_ls_R_factor_gt           0.049
_refine_ls_wR_factor_gt          0.049
_cod_data_source_file            EJSSIC-1991-28-867-881-2.cif
_cod_data_source_block           5
_cod_original_cell_volume        1716.2
_cod_database_code               4030344
Structure and bonding in the high molecular weight isopolymolybdate ion, [Mo36O112(H2O)16]8-. The crystal structure of Na8[Mo36O112(H2O)16].58H2O
Krebs, B.; Stiller, S.; Tytko, K. H.; Mehmke, J.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 883–903; doi:

data_4030345
_publ_section_title
;
 Structure and bonding in the high molecular weight isopolymolybdate ion,
 [Mo36O112(H2O)16]8-. The crystal structure of Na8[Mo36O112(H2O)16].58H2O
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              883
_journal_page_last               903
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'H148 Mo36 Na8 O186'
_chemical_formula_weight         6762.83
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-I 2ya'
_symmetry_space_group_name_H-M   'I 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.73(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   32.971(10)
_cell_length_b                   19.662(7)
_cell_length_c                   25.288(8)
_cell_volume                     16312(9)
_diffrn_ambient_temperature      173
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    27.8
_exptl_crystal_density_diffrn    2.753
_exptl_crystal_density_meas      2.71
_refine_ls_number_parameters     552
_refine_ls_number_reflns         12540
_refine_ls_R_factor_gt           0.088
_refine_ls_wR_factor_gt          0.079
_cod_data_source_file            EJSSIC-1991-28-883-903.cif
_cod_data_source_block           Na8Mo36O112
_cod_original_sg_symbol_H-M      'I 2/a'
_cod_database_code               4030345
Reductive Lithium Insertion into B-cation deficient Niobium Perovskite Oxides
Perejon, Antonio; Hayward, Michael Andrew; Dalton Trans.  (2014) –; doi:10.1039/C4DT03193H

data_7033424
_publ_section_title
;
 Reductive Lithium Insertion into B-cation deficient Niobium Perovskite
 Oxides
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C4DT03193H
_journal_year                    2014
_chemical_formula_sum            'Ba15 Li3 Nb12 O45'
_chemical_formula_weight         3915.578
_space_group_crystal_system      trigonal
_space_group_IT_number           166
_space_group_name_Hall           '-R 3 2"'
_space_group_name_H-M_alt        'R -3 m :H'
_audit_creation_date             2014-12-05T09:45:07
_cell_angle_alpha                90.000
_cell_angle_beta                 90.000
_cell_angle_gamma                120.000
_cell_formula_units_Z            3
_cell_length_a                   5.8012(3)
_cell_length_b                   5.8012(3)
_cell_length_c                   35.675(2)
_cell_volume                     1039.75(10)
_diffrn_ambient_temperature      298
_diffrn_radiation_type           neutron
_cod_data_source_file            c4dt03193h3.cif
_cod_data_source_block           added_by_encifer
_cod_original_cell_volume        1039.8(1)
_cod_original_formula_sum        'Ba15 Nb12 Li3 O45'
_cod_database_code               7033424
Novel layered structures in metal salts of bis(sulfonyl) methanes
Desmarteau, D. D.; Pennington, W. T.; Sung, K.-S.; Zhu, S.-Z.; Scott, R.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 905–917; doi:

data_4030346
_publ_section_title
;
 Novel layered structures in metal salts of bis(sulfonyl) methanes
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              905
_journal_page_last               917
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'C3 H F6 K O4 S2'
_chemical_formula_weight         318.28
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 119.61(4)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   25.66(2)
_cell_length_b                   5.204(5)
_cell_length_c                   16.395(8)
_cell_volume                     1903(3)
_diffrn_ambient_temperature      294
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    1.088
_exptl_crystal_density_diffrn    2.222
_exptl_crystal_F_000             1248
_refine_ls_number_reflns         1108
_refine_ls_R_factor_gt           0.0620
_refine_ls_wR_factor_gt          0.0816
_cod_data_source_file            EJSSIC-1991-28-905-917-1.cif
_cod_data_source_block           1
_cod_original_cell_volume        1903(2)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               4030346
Novel layered structures in metal salts of bis(sulfonyl) methanes
Desmarteau, D. D.; Pennington, W. T.; Sung, K.-S.; Zhu, S.-Z.; Scott, R.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 905–917; doi:

data_4030347
_publ_section_title
;
 Novel layered structures in metal salts of bis(sulfonyl) methanes
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              905
_journal_page_last               917
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'C H F2 K O4 S2'
_chemical_formula_weight         218.26
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.22(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.452(1)
_cell_length_b                   14.710(4)
_cell_length_c                   7.929(2)
_cell_volume                     634.2(3)
_diffrn_ambient_temperature      294
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    1.488
_exptl_crystal_density_diffrn    2.286
_exptl_crystal_F_000             432
_refine_ls_number_reflns         916
_refine_ls_R_factor_gt           0.0398
_refine_ls_wR_factor_gt          0.0604
_cod_data_source_file            EJSSIC-1991-28-905-917-2.cif
_cod_data_source_block           2
_cod_original_cell_volume        634.2(2)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4030347
Novel layered structures in metal salts of bis(sulfonyl) methanes
Desmarteau, D. D.; Pennington, W. T.; Sung, K.-S.; Zhu, S.-Z.; Scott, R.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 905–917; doi:

data_4030348
_publ_section_title
;
 Novel layered structures in metal salts of bis(sulfonyl) methanes
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              905
_journal_page_last               917
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'C3 H2 F6 O4 S2'
_chemical_formula_weight         280.19
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.79(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.429(1)
_cell_length_b                   9.240(2)
_cell_length_c                   9.298(2)
_cell_volume                     446.54(17)
_diffrn_ambient_temperature      294
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    0.689
_exptl_crystal_density_diffrn    2.084
_exptl_crystal_F_000             276
_refine_ls_number_reflns         827
_refine_ls_R_factor_gt           0.0392
_refine_ls_wR_factor_gt          0.0501
_cod_data_source_file            EJSSIC-1991-28-905-917-3.cif
_cod_data_source_block           3
_cod_original_sg_symbol_H-M      'P 21'
_cod_database_code               4030348
Halogen bridged Re6L8 units in octahedral cluster thenium chalcohalides
Perrin, A.; Leduc, L.; Sergent, M.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 919–931; doi:

data_4030349
_publ_section_title
;
 Halogen bridged Re6L8 units in octahedral cluster thenium chalcohalides
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              919
_journal_page_last               931
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Cl6 Re6 Se6'
_chemical_formula_weight         1803.72
_space_group_IT_number           64
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      64
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.892(2)
_cell_length_b                   11.286(5)
_cell_length_c                   11.310(4)
_cell_volume                     1773.2(10)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    53.531
_exptl_crystal_density_diffrn    6.717
_exptl_crystal_F_000             3008
_refine_ls_number_parameters     50
_refine_ls_number_reflns         707
_refine_ls_R_factor_gt           0.065
_refine_ls_wR_factor_gt          0.085
_cod_data_source_file            EJSSIC-1991-28-919-931.cif
_cod_data_source_block           Re6Se6Cl6
_cod_original_sg_symbol_Hall     '-C 2bc 2'
_cod_database_code               4030349
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030350
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 F9 Fe2 Rb'
_chemical_formula_weight         642.83
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.949(1)
_cell_length_b                   5.949(1)
_cell_length_c                   20.837(1)
_cell_volume                     638.64(15)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    18.248
_exptl_crystal_density_diffrn    5.015
_exptl_crystal_F_000             846
_refine_ls_number_reflns         526
_refine_ls_R_factor_gt           0.025
_refine_ls_wR_factor_gt          0.028
_cod_data_source_file            EJSSIC-1991-28-959-969-1.cif
_cod_data_source_block           Ba2RbFe2F9
_cod_original_cell_volume        638.6(3)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030350
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030351
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 Co2 Cs F9'
_chemical_formula_weight         696.43
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.931(1)
_cell_length_b                   5.931(1)
_cell_length_c                   21.318(4)
_cell_volume                     649.4(2)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    16.983
_exptl_crystal_density_diffrn    5.342
_exptl_crystal_F_000             906
_refine_ls_number_reflns         624
_refine_ls_R_factor_gt           0.024
_refine_ls_wR_factor_gt          0.025
_cod_data_source_file            EJSSIC-1991-28-959-969-2.cif
_cod_data_source_block           Ba2CsCo2F9
_cod_original_cell_volume        649.4(3)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030351
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030352
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 F9 K Ni2'
_chemical_formula_weight         602.14
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.775(1)
_cell_length_b                   5.775(1)
_cell_length_c                   20.756(1)
_cell_volume                     599.48(15)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    14.989
_exptl_crystal_density_diffrn    5.004
_exptl_crystal_F_000             804
_refine_ls_number_reflns         647
_refine_ls_R_factor_gt           0.036
_refine_ls_wR_factor_gt          0.039
_cod_data_source_file            EJSSIC-1991-28-959-969-3.cif
_cod_data_source_block           Ba2KNi2F9
_cod_original_cell_volume        599.5(2)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030352
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030353
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 F9 Ni2 Rb'
_chemical_formula_weight         648.51
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.801(1)
_cell_length_b                   5.801(1)
_cell_length_c                   20.994(2)
_cell_volume                     611.83(16)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    20.106
_exptl_crystal_density_diffrn    5.281
_exptl_crystal_F_000             858
_refine_ls_number_reflns         369
_refine_ls_R_factor_gt           0.032
_refine_ls_wR_factor_gt          0.038
_cod_data_source_file            EJSSIC-1991-28-959-969-4.cif
_cod_data_source_block           Ba2RbNi2F9
_cod_original_cell_volume        611.8(3)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030353
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030354
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 Cs F9 Ni2'
_chemical_formula_weight         695.95
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.855(1)
_cell_length_b                   5.855(1)
_cell_length_c                   21.209(9)
_cell_volume                     629.7(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    18.048
_exptl_crystal_density_diffrn    5.506
_exptl_crystal_F_000             912
_refine_ls_number_reflns         351
_refine_ls_R_factor_gt           0.021
_refine_ls_wR_factor_gt          0.025
_cod_data_source_file            EJSSIC-1991-28-959-969-5.cif
_cod_data_source_block           Ba2CsNi2F9
_cod_original_cell_volume        629.7(4)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030354
Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and their hexagonal layer structure
Herdtweck, E.; Kummer, S.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 959–969; doi:

data_4030355
_publ_section_title
;
 Cation-deficient perovskites Ba2A(I)M2(II)F9 (M(II) = Fe, Co, Ni, Zn) and
 their hexagonal layer structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              959
_journal_page_last               969
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Ba2 Cs F9 Zn2'
_chemical_formula_weight         709.35
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.905(1)
_cell_length_b                   5.905(1)
_cell_length_c                   21.279(9)
_cell_volume                     642.6(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    18.891
_exptl_crystal_density_diffrn    5.499
_exptl_crystal_F_000             924
_refine_ls_number_reflns         338
_refine_ls_R_factor_gt           0.030
_refine_ls_wR_factor_gt          0.038
_cod_data_source_file            EJSSIC-1991-28-959-969-6.cif
_cod_data_source_block           Ba2CsZn2F9
_cod_original_cell_volume        642.6(4)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4030355